| Element    | Standard used | BG-1 (wt.%) | BG-1 (wt.%) | BG-1 (wt.%)  | BG-1 (wt.%)  | BG-2 (wt.%) | BG-2 (wt.%) | BG-2 (wt.%)  | BG-2 (wt.%)  | BG-3 (wt.%) | BG-3 (wt.%) | BG-3 (wt.%)  | BG-3 (wt.%)  |
| Element    | Standard used | Before      | Before      | After 14days | After 14days | Before      | Before      | After 14days | After 14days | Before      | Before      | After 14days | After 14days |
| Element    | Standard used | Avg.        | +-Er%x10    | Avg.         | +-Er%x10     | Avg.        | +-Er%x10    | Avg.         | +-Er%x10     | Avg.        | +-Er%x10    | Avg.         | +-Er%x10     |
| C          | CaCO3         | 14.6        | 0.02        | 16.44        | 0.024        | 14.45       | 0.031       | 16.44        | 0.01         | 9.62        | 0.031       | 13.01        | 0.039        |
| O          | SiO2          | 48.59       | 0.03        | 47.02        | 0.032        | 49.72       | 0.034       | 49.11        | 0.04         | 48.35       | 0.041       | 49.01        | 0.021        |
| Na         | Albite        | 12.97       | 0.025       | 8.48         | 0.031        | 8.48        | 0.023       | 6.48         | 0.028        | 2.63        | 0.031       | 1.13         | 0.041        |
| Mg         | MgO           | 2.78        | 0.031       | 3.28         | 0.034        | 3.28        | 0.025       | 3.28         | 0.032        | 0.54        | 0.029       | 0.41         | 0.031        |
| Si         | SiO2          | 14.65       | 0.032       | 14.12        | 0.031        | 14.12       | 0.027       | 13.12        | 0.031        | 23.51       | 0.028       | 18.47        | 0.021        |
| P          | GaP           | 1.96        | 0.031       | 2.51         | 0.032        | 2.68        | 0.041       | 3.12         | 0.049        | 4.54        | 0.05        | 4.98         | 0.043        |
| Ca         | Wollastonite  | 2.11        | 0.021       | 4.21         | 0.041        | 3.13        | 0.048       | 5.31         | 0.042        | 4.92        | 0.031       | 8.8          | 0.029        |
| Zn         | Zn            | 2.34        | 0.021       | 4.14         | 0.01         | 4.14        | 0.014       | 3.14         | 0.021        | 5.89        | 0.018       | 4.23         | 0.022        |
| Ca/P ratio | Ca/P ratio    | 1.07        | 1.07        | 1.68         | 1.68         | 1.17        | 1.17        | 1.7          | 1.7          | 1.08        | 1.08        | 1.77         | 1.77         |

Caption: Weight percentage of the elements of samples from EDX data. EDX results are average (Avg.) of 5 measurements and the observed error (Er) percentage is also presented.

You are provided with a table from a material science paper. Here are JSON templates for two types of numeric cells: "Other" and "Glass_Compound_Amount":
{"value": "xx", "type": "Other"}
{"value": "xx", "type": "Glass_Compound_Amount", "constituent": "xx", "unit": "xx", "material": "xx"}

Please describe all numeric cells in the above table following the JSON templates (proceeding by row in a left-right, top-down direction). For each cell, output one JSON description per line. For any unanswerable attributes in the templates, set their value to the placeholder "xx".

Cell Description:
{"value": "14.6", "type": "Glass_Compound_Amount", "constituent": "C", "unit": "wt", "material": "BG-1 (wt.%)"}
{"value": "0.02", "type": "Other"}
{"value": "16.44", "type": "Glass_Compound_Amount", "constituent": "C", "unit": "wt", "material": "BG-1 (wt.%)"}
{"value": "0.024", "type": "Other"}
{"value": "14.45", "type": "Glass_Compound_Amount", "constituent": "C", "unit": "wt", "material": "BG-2 (wt.%)"}
{"value": "0.031", "type": "Other"}
{"value": "16.44", "type": "Glass_Compound_Amount", "constituent": "C", "unit": "wt", "material": "BG-2 (wt.%)"}
{"value": "0.01", "type": "Other"}
{"value": "9.62", "type": "Glass_Compound_Amount", "constituent": "C", "unit": "wt", "material": "BG-3 (wt.%)"}
{"value": "0.031", "type": "Other"}
{"value": "13.01", "type": "Glass_Compound_Amount", "constituent": "C", "unit": "wt", "material": "BG-3 (wt.%)"}
{"value": "0.039", "type": "Other"}
{"value": "48.59", "type": "Glass_Compound_Amount", "constituent": "O", "unit": "wt", "material": "BG-1 (wt.%)"}
{"value": "0.03", "type": "Other"}
{"value": "47.02", "type": "Other"}
{"value": "0.032", "type": "Other"}
{"value": "49.72", "type": "Other"}
{"value": "0.034", "type": "Other"}
{"value": "49.11", "type": "Other"}
{"value": "0.04", "type": "Other"}
{"value": "48.35", "type": "Other"}
{"value": "0.041", "type": "Other"}
{"value": "49.01", "type": "Other"}
{"value": "0.021", "type": "Other"}
{"value": "12.97", "type": "Glass_Compound_Amount", "constituent": "Na", "unit": "wt", "material": "BG-1 (wt.%)"}
{"value": "0.025", "type": "Other"}
{"value": "8.48", "type": "Other"}
{"value": "0.031", "type": "Other"}
{"value": "8.48", "type": "Other"}
{"value": "0.023", "type": "Other"}
{"value": "6.48", "type": "Other"}
{"value": "0.028", "type": "Other"}
{"value": "2.63", "type": "Other"}
{"value": "0.031", "type": "Other"}
{"value": "1.13", "type": "Other"}
{"value": "0.041", "type": "Other"}
{"value": "2.78", "type": "Glass_Compound_Amount", "constituent": "Mg", "unit": "wt", "material": "BG-1 (wt.%)"}
{"value": "0.031", "type": "Other"}
{"value": "3.28", "type": "Other"}
{"value": "0.034", "type": "Other"}
{"value": "3.28", "type": "Other"}
{"value": "0.025", "type": "Other"}
{"value": "3.28", "type": "Other"}
{"value": "0.032", "type": "Other"}
{"value": "0.54", "type": "Other"}
{"value": "0.029", "type": "Other"}
{"value": "0.41", "type": "Other"}
{"value": "0.031", "type": "Other"}
{"value": "14.65", "type": "Glass_Compound_Amount", "constituent": "Si", "unit": "wt", "material": "BG-1 (wt.%)"}
{"value": "0.032", "type": "Other"}
{"value": "14.12", "type": "Other"}
{"value": "0.031", "type": "Other"}
{"value": "14.12", "type": "Other"}
{"value": "0.027", "type": "Other"}
{"value": "13.12", "type": "Other"}
{"value": "0.031", "type": "Other"}
{"value": "23.51", "type": "Other"}
{"value": "0.028", "type": "Other"}
{"value": "18.47", "type": "Other"}
{"value": "0.021", "type": "Other"}
{"value": "1.96", "type": "Glass_Compound_Amount", "constituent": "P", "unit": "wt", "material": "BG-1 (wt.%)"}
{"value": "0.031", "type": "Other"}
{"value": "2.51", "type": "Other"}
{"value": "0.032", "type": "Other"}
{"value": "2.68", "type": "Other"}
{"value": "0.041", "type": "Other"}
{"value": "3.12", "type": "Other"}
{"value": "0.049", "type": "Other"}
{"value": "4.54", "type": "Other"}
{"value": "0.05", "type": "Other"}
{"value": "4.98", "type": "Other"}
{"value": "0.043", "type": "Other"}
{"value": "2.11", "type": "Glass_Compound_Amount", "constituent": "Ca", "unit": "wt", "material": "BG-1 (wt.%)"}
{"value": "0.021", "type": "Other"}
{"value": "4.21", "type": "Other"}
{"value": "0.041", "type": "Other"}
{"value": "3.13", "type": "Other"}
{"value": "0.048", "type": "Other"}
{"value": "5.31", "type": "Other"}
{"value": "0.042", "type": "Other"}
{"value": "4.92", "type": "Other"}
{"value": "0.031", "type": "Other"}
{"value": "8.8", "type": "Other"}
{"value": "0.029", "type": "Other"}
{"value": "2.34", "type": "Glass_Compound_Amount", "constituent": "Zn", "unit": "wt", "material": "BG-1 (wt.%)"}
{"value": "0.021", "type": "Other"}
{"value": "4.14", "type": "Glass_Compound_Amount", "constituent": "Zn", "unit": "wt", "material": "BG-1 (wt.%)"}
{"value": "0.01", "type": "Other"}
{"value": "4.14", "type": "Glass_Compound_Amount", "constituent": "Zn", "unit": "wt", "material": "BG-2 (wt.%)"}
{"value": "0.014", "type": "Other"}
{"value": "3.14", "type": "Glass_Compound_Amount", "constituent": "Zn", "unit": "wt", "material": "BG-2 (wt.%)"}
{"value": "0.021", "type": "Other"}
{"value": "5.89", "type": "Glass_Compound_Amount", "constituent": "Zn", "unit": "wt", "material": "BG-3 (wt.%)"}
{"value": "0.018", "type": "Other"}
{"value": "4.23", "type": "Glass_Compound_Amount", "constituent": "Zn", "unit": "wt", "material": "BG-3 (wt.%)"}
{"value": "0.022", "type": "Other"}
{"value": "1.07", "type": "Other"}
{"value": "1.07", "type": "Other"}
{"value": "1.68", "type": "Other"}
{"value": "1.68", "type": "Other"}
{"value": "1.17", "type": "Other"}
{"value": "1.17", "type": "Other"}
{"value": "1.7", "type": "Other"}
{"value": "1.7", "type": "Other"}
{"value": "1.08", "type": "Other"}
{"value": "1.08", "type": "Other"}
{"value": "1.77", "type": "Other"}
{"value": "1.77", "type": "Other"}